Compressive strength of concrete cube take a look at provides an inspiration regarding all the characteristics of concrete. By this single take a look at one choose that whether or not Concreting has been done properly or not. Concrete compressive strength for general construction varies from fifteen MPa (2200 psi) to 30 MPa (4400 psi) and better in industrial and industrial structures.
Compressive strength of concrete depends on several factors like water-cement magnitude relation, cement strength, quality of concrete material, internal control throughout production of concrete etc.
Test for compressive strength is distributed either on cube or cylinder. numerous customary codes recommends concrete cylinder or concrete cube because the standard specimen for the take a look at. yankee Society for take a look ating Materials ASTM C39/C39M provides customary Test technique for Compressive Strength of Cylindrical Concrete Specimens.
Compressive Strength Definition:
Compressive strength is that the ability of fabric or structure to hold the masses on its surface with none crack or deflection. a fabric beneath compression tends to scale back the dimensions, whereas in tension, size elongates.
Compressive Strength Formula:
Compressive strength formula for any material is that the load applied at the purpose of failure to the crosswise space of the face on that load was applied.
Compressive Strength = Load / Cross-sectional Area
Procedure: Compressive Strength Test of Concrete Cubes
For cube test two types of specimens either cubes of 15cm X 15cm X 15cm or 10cm X 10cm x 10cm depending upon the size of aggregate are used. For most of the works cubical moulds of size 15cm x 15cm x 15cm are commonly used.
This concrete is poured in the mould and tempered properly so as not to have any voids. After 24 hours these moulds are removed and test specimens are put in water for curing. The top surface of these specimen should be made even and smooth. This is done by putting cement paste and spreading smoothly on whole area of specimen.
These specimens are tested by compression testing machine after 7 days curing or 28 days curing. Load should be applied gradually at the rate of 140 kg/cm2 per minute till the Specimens fails. Load at the failure divided by area of specimen gives the compressive strength of concrete.
Following are the procedure for testing Compressive strength of Concrete Cubes
Apparatus for Concrete Cube Test
Compression testing machine
Preparation of Concrete Cube Specimen
The proportion and material for making these test specimens are from the same concrete used in the field.
6 cubes of 15 cm size Mix. M15 or above
Mixing of Concrete for Cube Test
Mix the concrete either by hand or in a laboratory batch mixer
- Mix the cement and fine aggregate on a water tight none-absorbent platform until the mixture is thoroughly blended and is of uniform color
- Add the coarse aggregate and mix with cement and fine aggregate until the coarse aggregate is uniformly distributed throughout the batch
- Add water and mix it until the concrete appears to be homogeneous and of the desired consistency
Sampling of Cubes for Test
- Clean the mounds and apply oil
- Fill the concrete in the molds in layers approximately 5 cm thick
- Compact each layer with not less than 35 strokes per layer using a tamping rod (steel bar 16mm diameter and 60cm long, bullet pointed at lower end)
- Level the top surface and smoothen it with a trowel
Curing of Cubes
The test specimens are stored in moist air for 24 hours and after this period the specimens are marked and removed from the molds and kept submerged in clear fresh water until taken out prior to test.
Precautions for Tests
The water for curing should be tested every 7 days and the temperature of water must be at 27+-2oC.
Procedure for Concrete Cube Test
- Remove the specimen from water after specified curing time and wipe out excess water from the surface.
- Take the dimension of the specimen to the nearest 0.2m
- Clean the bearing surface of the testing machine
- Place the specimen in the machine in such a manner that the load shall be applied to the opposite sides of the cube cast.
- Align the specimen centrally on the base plate of the machine.
- Rotate the movable portion gently by hand so that it touches the top surface of the specimen.
- Apply the load gradually without shock and continuously at the rate of 140 kg/cm2/minute till the specimen fails
- Record the maximum load and note any unusual features in the type of failure.
Minimum three specimens should be tested at each selected age. If strength of any specimen varies by more than 15 percent of average strength, results of such specimen should be rejected. Average of three specimens gives the crushing strength of concrete. The strength requirements of concrete.
Calculations of Compressive Strength
Size of the cube =15cmx15cmx15cm
Area of the specimen (calculated from the mean size of the specimen )=225 cm2
Characteristic compressive strength(f ck)at 7 days =
Expected maximum load =fck x area x f.s
Range to be selected is …………………..
Similar calculation should be done for 28 day compressive strength
Maximum load applied =……….tones = ………….N
Compressive strength = (Load in N/ Area in mm2)=……………N/mm2
Reports of Cube Test
- Identification mark
- Date of test
- Age of specimen
- Curing conditions, including date of manufacture of specimen
- Appearance of fractured faces of concrete and the type of fracture if they are unusual
Results of Concrete Cube Test
Average compressive strength of the concrete cube = ………….N/ mm2 (at 7 days)
Average compressive strength of the concrete cube =………. N/mm2 (at 28 days)
Compressive Strength of Concrete at Various Ages
The strength of concrete increases with age. Table shows the strength of concrete at different ages in comparison with the strength at 28 days after casting.
Compressive Strength of Different Grades of Concrete at 7 and 28 Days
|Grade of Concrete||Minimum compressive strength N/mm2 at 7 days||Specified characteristic compressive strength (N/mm2) at 28 days|